Feb 20, 2013 - The triplet superconducting correlations can carry spin-polarized supercurrents, i.e. currents without dissipation, that can be exploited in several ways in ...... 61 A. V. Burmistrova, I. A. Devyatov, Alexander A. Golubov, Keiji Yada,
Oct 6, 2008 - subwavelength nanodevices the electronic quantum transport properties present deep analogies with classical phenomena of subwavelength optics. By introducing the concept of electronic diffraction barrier to represent the ..... the Dirac
reversibly altered so as to switch the atom's electronic configuration between low-spin (LS) and high-spin (HS) states. ... SCO molecules have provided phenomenological modelling of experimental transport data to support a .... We find that, at room
For small E, provided t, r are slowly varying compared with (E/EF )kF L, one may evaluate r, t at E = 0 and write Â¯tâ tâ and Â¯r â râ. This yields equations (8) to ...
Aharonov-Bohm type oscillations superimposed on the first commensurability peak.5,6 The search for an artifi- cial band structure at B=0 T is still ongoing. ..... 12 Min Ouyang and David D. Awschalom, Science 301, 1074. (2003). 13 N. Y. Morgan, C. A.
Feb 15, 2016 - SQUID magnetometer was driven by an arbitrary wave- form generator ..... mechanism which contributes â 20 % to the total pen- etrated flux.
A.F. Volkov. Theoretische Physik III, Ruhr-UniversitÃ¤t Bochum, D-44780 Bochum, Germany and. Institute of Radioengineering and Electronics of the Russian Academy of Sciences, 125009 Moscow, Russia. (Dated: November 12, 2017). We report superconductin
Feb 1, 2008 - conductance minimum at zero voltage V = 0 and a peak at eV â â, where â is the superconducting energy gap. In the experiment of Kastalskii et al. ..... the above two expressions refer to a two-probe and to a four-probe measurement
HI = HD + HR + HRD tun . (2). HI is the Hamiltonian of the interferometer, HL and HR describe the leads and the trun- cated ring, i.e. what is left from it after removing the dots (the ... Actually the effective Hamiltonian of the dot has resonances
Feb 1, 2008 - [tii(pF , pF ), gâ,i. (pF )]âÎ´(R â Rc). (2). Here Rc is the position of the contact and vF is the Fermi velocity at point pF on the Fermi surface. The Green's function gâ,i is an intermediate Green's function ob- ..... The scal
Jul 17, 2013 - address transport robustness in natural light harvesting complexes. INTRODUCTION. Transport of charge or ... ted, coherent behavior results in enhanced transport as compared to incoherent (particle like) ...... Complex network analysis
Jul 21, 2006 - quantum information applications as charge and spin qubits1. Recently ... evidence that transport through this system is coherent when all three ...
We apply a first-principles computational approach to study a light-sensitive molecular switch. The molecule that comprises the switch can convert between a trans and a cis configuration upon photo-excitation. We find that the conductance of the two
Feb 14, 2006 - We report an insulator-metal-insulator transition in films of five metal phthalocyanines ... nines as a model class of compounds for the controlled.
Eq. (2.27)], goes back to the invariant measure (2.21), as it should. Secondly, we obstruct the right lead by making the barrier there a perfect reflector. ..... route, taking advantage of the Jacobian between unre- stricted S matrices that we alread
Jun 7, 2018 - Semiconducting carbon nanotubes (CNTs) are promis- ing candidates for ..... diffusion equation with an additional sink term, which traps the ...
Feb 14, 2012 - value is 170 Ry for the real-space grid. ... where T(E,Vb) is the transmission probability of electrons incident at an energy E from the left to .... electrode, since the state is well localized in a region controlled by the left lead.
Dec 1, 1998 - to the energy average of S which, through the notion of ergodicity, is expressed as the average over an ensemble of .... electronic transport through ballistic chaotic cavities, or ballistic quantum dots, described in section ... phase
For two concentric nanotubes symmetry breaking can reduce the maximum intertube conductance from 4e2/h to 2e2/h. The phenomena discussed here can serve as a foundation for building nanotube electronic circuits and high speed nanoscale electromechanic
Aug 27, 2010 - have a complementary behavior, that we study and analyze by means of a tight-binding method and a continuum Dirac model. ... nar geometry by cutting graphene layers.13 Another way to modify the band structure of ... ties of bilayer arm
Long distance electron transfer (ET) plays an important part in many biological processes. Also, .... These data may be available under moderate electronic.
Feb 14, 2006 - 5CREST, Japan Science and Technology Corporation Kawaguchi ... orbital degeneracy in MPc, our findings are of interest in the study of ...
Feb 3, 2014 - are compared with those from several other approaches for a wide range of parameters. ..... For comparison we also show in these plots the corresponding results ob- tained by the interpolative self-energy approach (ISA) of. Ref.  an
Jun 9, 2010 - hilation of topological defects, similar to those discussed by the Kibble-Zurek .... 3b) we first plot the spatially homogeneous solution with Î¾ = 0, with and without the P pulse. In this particular simulation, the parameters were chos
Coherent electronic transport through a superconducting film M. Boˇzovi´c, Z. Pajovi´c, and Z. Radovi´c
arXiv:cond-mat/0209355v2 [cond-mat.supr-con] 24 Jan 2003
Department of Physics, University of Belgrade, P.O. Box 368, 11001 Belgrade, Yugoslavia We study coherent quantum transport through a superconducting film connected to normal-metal electrodes. Simple expressions for the differential conductance and the local density of states are obtained in the clean limit and for transparent interfaces. Quasiparticle interference causes periodic vanishing of the Andreev reflection at the energies of geometrical resonances, subgap transport, and gapless superconductivity near the interfaces. Application of the results to spectroscopic measurements of the superconducting gap and the Fermi velocity is analyzed.
Conducting properties of normal metal/superconductor/normal metal (NSN) heterostructures have attracted considerable interest.1,2 Electronic transport through a normal metal/superconductor (NS) junction, with an insulating barrier of arbitrary strength at the interface, was studied by Blonder, Tinkham, and Klapwijk (BTK),3 and the Andreev reflection4 was recognized as the mechanism of normal-to-supercurrent conversion.5,6 The BTK model can be used when electrons pass incoherently through the interfaces of NSN double junctions.7 However, in clean superconducting heterostructures coherent quantum transport is strongly influenced by size effects due to the interplay between geometrical resonances and the Andreev reflection.8,9,10 Well-known examples are the current-carrying Andreev bound states11,12 and multiple Andreev reflections13,14,15 in superconductor/normal metal/superconductor (SNS) junctions. Since early experiments by Tomasch,16 the geometric resonance nature of the differential conductance oscillations in SNS and NSN tunnel junctions has been attributed to the electron interference in the central layer.17,18,19,20 Recently, McMillan-Rowell oscillations were observed in SNS tunnel junctions of d-wave superconductors, and used in measurements of the superconducting gap and the Fermi velocity.21 In this paper, we focus on size and coherency effects in NSN double junctions with a clean conventional (s-wave) superconductor and transparent interfaces. In that case, instead of a fully numerical treatment,8,22 a simple analytic form for the differential conductance and the local quasiparticle density of states (DOS) can be obtained from the solution of the Bogoliubov-de Gennes equation. The proximity effect, which is significant in thin superconducting films, is taken into account through the self-consistent calculation of the pair potential. Striking consequence of the quasiparticle interference in the clean metallic NSN junctions include periodic vanishing of the Andreev reflection at the energies of geometrical resonances and the characteristic changes of DOS with respect to the bulk superconductor. II.
We consider an NSN double junction consisting of a clean superconducting layer of thickness d, connected to normal-metal electrodes by transparent interfaces. The quasiparticle propagation is described by the Bogoliubov–de Gennes equation u(r) u(r) H0 (r) ∆(r) , (1) = E v(r) v(r) ∆∗ (r) −H0 (r) with H0 (r) =p −~2 ∇2 /2m − EF , where EF is the Fermi energy. For simplicity, the magnitude of the Fermi wave vector, kF = 2mEF /~2 , is assumed to be constant through the junction. The superconducting pair potential is taken in the form ∆(r) = ∆Θ(z)Θ(l − z), where Θ(z) is the Heaviside step function, and the z-axis is perpendicular to the layers. In Eq. (1), E is the quasiparticle energy with respect to the Fermi level. The electron effective mass m is assumed to be the same for the entire junction. The parallel component of the wave vector k|| is conserved, and the wave function u(r) = exp(ik|| · r) ψ(z), (2) v(r) satisfies the continuity boundary conditions for ψ(z) and ψ ′ (z) at z = 0 and z = d. The four independent solutions of Eq. (1) correspond to the four types of injection: an electron or a hole, from either the left or the right electrode.6
2 For the injection of an electron from the left, with energy E > 0 and angle of incidence θ (measured from the z-axis), solution for ψ(z) has the following form 0 1 − + z < 0, + a(E, θ) exp(ik z) exp(ik z) 1 0 v¯ u ¯ − + (3) 0 < z < d, + b2 (E, θ) exp(iq z) ψ(z) = b1 (E, θ) exp(iq z) u ¯ v ¯ c(E, θ) exp(ik + z) 1 z > d. 0 p p √ 2 2 Here, u ¯ = (1 + Ω/E)/2 and v¯ = (1 − Ω/E)/2 are the BCS coherence factors, q q and Ω = E − ∆ . The z(2m/~2 )(EF ± E) − k2|| and q ± = (2m/~2 )(EF ± Ω) − k2|| , where components of the wave vectors are k ± = p |k|| | = (2m/~2 )(EF + E) sin θ. The coefficients a and c are, respectively, the probability amplitudes of the Andreev reflection as a hole of the opposite spin (AR) and transmission to the right electrode as an electron (TE). The amplitudes of the Bogoliubov electron-like and hole-like quasiparticles, propagating in the superconducting layer, are given by the coefficients b1 and b2 . The normal reflection of electrons and the transmission to the right electrode as a hole are absent. Solutions for the general case of insulating interfaces and the Fermi velocity mismatch are given in Ref. 7. By neglecting the small terms E/EF ≪ 1 and ∆/EF ≪ 1 in the wave vectors, except in the exponent (4) ζ = d q+ − q− , solutions of the boundary-condition equations can be written in a simple form: a(E, θ) = u¯v¯[1 − exp(iζz/d)]/[¯ u2 − 2 2 2 2 2 v¯ exp(iζz/d)], b1 (E, θ) = u¯/[¯ u − v¯ exp(iζz/d)], b2 (E, θ) = −¯ v exp(iζz/d)/[¯ u − v¯ exp(iζz/d)], and c(E, θ) = −i(¯ u2 − 2 2 2 v¯ ) exp(iζz/d)/[¯ u − v¯ exp(iζz/d)]. From the probability current conservation, the probabilities of outgoing particles satisfy the normalization condition A(E, θ) + C(E, θ) = 1, where A(E, θ) = |a(E, θ)|2 and C(E, θ) = |c(E, θ)|2 . Explicitly, the AR probability is 2 ∆ sin(ζ/2) . (5) A(E, θ) = E sin(ζ/2) + iΩ cos(ζ/2)
Solutions for the other three types of injection can be obtained by the same procedure. In particular, if a hole with energy −E and angle of incidence θ is injected from the left, the substitution q + ⇋ q − holds, and the scattering probabilities are the same as for the injection of an electron with E and θ. Therefore, in order to include the description of both electron and hole injection, the calculated probabilities should be regarded as even functions of E. Also, for an electron or a hole injected from the right, the probabilities are the same as for the injection from the left. From Eq. (5), it follows that A(E, θ) = 0, and consequently C(E, θ) = 1, when ζ = 2nπ
for n = 0, ±1, ±2, . . .. Therefore, the Andreev reflection vanishes, and the electron transmission becomes complete (without creation or annihilation of Cooper pairs), at the energies of geometrical resonances in the quasiparticle spectrum, given by Eq. (6). For thin superconducting films, the proximity effect is important and the self-consistent treatment of the pair potential is required. However, the spatial variation of the pair potential is negligible for d/ξ0 . 1, where ξ0 = ~vF /π∆0 is the BCS coherence length in the bulk superconductor, and we can use the previous solution with the step-like form for ∆. The pair potential is given by the self-consistency equation Z Z ~ωD dΩ u(r)v ∗ (r) tanh(E/2kB T ), (7) ∆(z) = 2λN (0) d2 k|| 0
where λ is the BCS coupling constant and N (0) = mkF /2π 2 ~2 is the normal-metal density of states (per spin) at the Fermi level. We calculate the spatial average of ∆(z) using the standard iteration procedure Z 1 d ∆i+1 = ∆i (z)dz, (8) d 0 p by setting Ω = E 2 − ∆2i in Eq. (7) in order to obtain ∆i (z) in the i-th iteration.23 Starting from the bulk value ∆0 , we repeat this procedure until the difference between ∆i+1 and ∆i becomes sufficiently small. In Fig. 1, we show the resulting ∆ as a function of d, at zero temperature.
DIFFERENTIAL CONDUCTANCE AND DENSITY OF STATES
The normalized differential conductance at zero temperature for a planar double junction is Z π/2 G(E) = dθ sin θ cos θ [1 + A(E, θ)] , GN 0
where GN = e2 /h. In the one-dimensional (1D) case, the normalized differential conductance is simply g(E) = 1 + A(E, 0). GN
Coherent transport through an NSN double junction is influenced by considerable changes of the quasiparticle density of states with respect to the bulk superconductor.17,18 Adopting the method introduced by McMillan,19 Ishii,5 and Furusaki and Tsukada,6 we evaluate the Green functions by combining the solutions of the Bogoliubov-de Gennes equation. From the imaginary part of the retarded Green function, we obtain the local value of the partial density of states (PDOS) for the superconducting film, normalized with respect to the 1D normal-metal density of states per spin at the Fermi level, n 1 ˜ (z, θ, E) = N Re 2E 2 (E 2 + Ω2 ) + 2E 2 ∆2 cos ζ Γ(E) cos θ +[cos(ζ(z/d − 1)) + cos(ζz/d)][∆4 − ∆2 (E 2 + Ω2 ) cos ζ] o +2E 2 ∆2 [sin(ζ(z/d − 1)) − sin(ζz/d)] sin ζ ,
where Γ(E) = [(E 2 + Ω2 ) cos ζ − ∆2 ]2 + 4E 2 Ω2 sin2 ζ. For a planar junction, the local DOS for the superconducting film is given by Z π/2 N (z, E) ˜ (z, θ, E). = dθ sin θ cos θ N N (0) 0
˜ (z, θ, E) = N (z, E)/N (0) = 1 in the normal-metal electrodes (z < 0 and z > d). Here, N Characteristic features of the coherence in NSN double junctions are subgap transport of electrons and oscillations of the conductance. Due to the interference effect, the Andreev reflection is suppressed for E < ∆, whereas the AR probability oscillates with E and d, for E > ∆. The subgap transport is dominant in thin superconducting films, and the oscillatory behavior is apparent in thick films. These oscillations are more pronounced in the 1D case, which is shown in Fig. 2. It can be clearly seen that the positions of the minima in g(E) exactly match the positions of the maxima in PDOS, corresponding to the geometrical resonances imposed by Eq. (6). Results can be applied to spectroscopic measurements of ∆ and vF . From Eq. (6) for θ = 0, the energies of the geometrical resonances, En , satisfy π~v 2 F En2 = ∆2 + n2 , (14) d 2 2 2 where n = 1, 2, . . . counts the conductance minima. Therefore, the plot of En vs n has the intercept equal to ∆ , −1 2 and the slope equal to tan (π~vF /d) . An example is shown in the Inset of Fig. 2. Note that the points obtained from the minima of G(E) follow practically the same linear law as those of g(E). The obtained results are in a strong contrast with the conductance spectrum and DOS of tunnel junctions. In the latter case, g(E) and PDOS reduce to δ-function-like spikes at the bound state energies of the isolated superconducting film, given by lq + = n1 π and lq − = n2 π, where n1 − n2 = 2n, with n given in Eq. (6).24 The conductance spectra G(E)/GN and the local DOS for the superconducting film in a planar NSN double junction are illustrated in Figs. 3 and 4, for d/ξ0 = 1 and d/ξ0 = 10, using the self-consistent pair potential ∆/∆0 = 0.816 and ∆/∆0 = 1, respectively. In Fig. 3, the conductance spectra are compared to the BTK result describing the incoherent transport. It can be seen in Fig. 4(a) that the energy spectrum of a thin superconducting film is practically gapless. For a thick superconducting film, this is the case only near the interfaces, Fig. 4(b). The characteristic oscillations of the local DOS become more apparent for a thick film. The oscillations of G(E) and of the local DOS are not completely smeared in the 3D case. The positions of the minima in G(E) or the maxima of the local DOS are still close to the positions of the resonant quasiparticle states in the 1D case.
We have derived simple expressions describing the finite size and coherency effects in the metallic NSN double junctions, suitable for experimental data analysis. The main features of the coherent quantum transport through a superconducting film are subgap transport and oscillations of the differential conductance. The Andreev reflection is suppressed below the gap, especially in thin films. The conductance oscillates as a function of the layer thickness and of the quasiparticle energy above the superconducting gap. Periodic vanishing of the Andreev reflection at the energies of geometrical resonances is an important consequence of the quasiparticle interference; the conductance minima correspond to the maxima in the density of states. Measurements of the conductance spectra of metallic NSN double junctions could be used for accurate determination of the pair potential and the Fermi velocity in superconductors. We are grateful to Ivan Boˇzovi´c for useful discussions. This work has been supported by the Serbian Ministry of Science, Technology, and Development, Project N◦ 1899.
C. W. J. Beenakker, Rev. Mod. Phys. 69, 731 (1997). I. Nevirkovets, J. B. Ketterson, and S. Lomatch, Appl. Phys. Lett. 74, 1624 (1999). G. E. Blonder, M. Tinkham, and T. M. Klapwijk, Phys. Rev. B 25, 4515 (1982). ´ A. F. Andreev, Zh. Eksp. Teor. Fiz. 46, 1823 (1964) [Sov. Phys. JETP 19, 1228 (1964)]. C. Ishii, Prog. Theor. Phys. 44, 1525 (1970). A. Furusaki and M. Tsukada, Solid State Commun. 78, 299 (1991). Z. Zheng, D. Y. Xing, G. Sun, and J. Dong, Phys. Rev. B 62, 14 326 (2000). J. S´ anchez-Ca˜ nizares and F. Sols, Physica B 252, 304 (1998). A. Brinkman and A. A. Golubov, Phys. Rev. B 61, 11 297 (1999). M. Boˇzovi´c and Z. Radovi´c, Phys. Rev. B 66, 134524 (2002). ˇ O. Sipr and B. L. Gy¨ orffy, J. Phys: Condens. Matter 8, 169 (1996). S. Kashiwaya and Y. Tanaka, Rep. Prog. Phys. 63, 1641 (2000). T. M. Klapwijk, G. E. Blonder, and M. Tinkham, Physica B 109-110, 1657 (1982). T. Hoss, C. Strunk, T. Nussbaumer, R. Huber, U. Staufer, and C. Sch¨ onenberger, Phys. Rev. B 62, 4079 (2000). ˚ A. Ingerman, G. Johansson, V. S. Shumeiko, and G. Wendin, Phys. Rev. B 64, 144504 (2001). W. J. Tomasch, Phys. Rev. Lett. 15, 672 (1965); ibid. 16, 16 (1966). W. L. McMillan and P. W. Anderson, Phys. Rev. Lett. 16, 85 (1966). J. M. Rowell and W. L. McMillan, Phys. Rev. Lett. 16, 453 (1966). W. L. McMillan, Phys. Rev. 175, 559 (1968). J. Demers and A. Griffin, Can. J. Phys. 49, 285 (1971). O. Nesher and G. Koren, Phys. Rev. B 60, 9287 (1999). B. P. Stojkovi´c and O. T. Valls, Phys. Rev. B 47, 5922 (1993); ibid. 50, 3374 (1994). Y. Tanaka and M. Tsukada, Phys. Rev. B 44, 7578 (1991). See Fig. 2 in M. Boˇzovi´c and Z. Radovi´c, cond-mat/0207375 (2002). FIG. 1: The pair potential ∆ as a function of the film thickness d, at zero temperature.
˜ (d/2, 0, E), for d/ξ0 = 10. Inset: FIG. 2: (a) Partial (θ = 0) conductance spectra, g(E)/GN , and (b) corresponding PDOS, N square of resonant energies, En2 , vs n2 obtained from the minima of g(E) (open circles) and G(E) (full squares). FIG. 3: Differential conductance spectra G(E)/GN for d/ξ0 = 1 and 10 (solid curves). The BTK result is shown for comparison (dashed curve). FIG. 4: Local DOS, N (z, E)/N (0), for z = d/2 (solid curves) and z = 0 or d (dotted curves) as a function of E/∆0 is shown for d/ξ0 = 1 (a), and d/ξ0 = 10 (b).